LMucko/crystallography-open-database huggingface dataset:
Combined neutron powder and X-ray single-crystal diffraction refinement of the atomic structure and hydrogen bonding of goslarite (ZnSO4*7H2O) Note: Combined neutron powder X-ray refinement
Anderson, J. L.; Peterson, R. C.; Swaison, I. P.; Mineralogical Magazine 69 (2005) 259–271; doi:

data_9017541
_publ_section_title
;
 Combined neutron powder and X-ray single-crystal diffraction refinement of the
 atomic structure and hydrogen bonding of goslarite (ZnSO4*7H2O)
 Note: Combined neutron powder X-ray refinement
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              259
_journal_page_last               271
_journal_volume                  69
_journal_year                    2005
_chemical_compound_source        Synthetic
_chemical_formula_sum            'H14 O11 S Zn'
_chemical_name_mineral           Goslarite
_space_group_IT_number           19
_space_group_name_Hall           'P 2ac 2ab'
_space_group_name_H-M_alt        'P 21 21 21'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.8176
_cell_length_b                   12.0755
_cell_length_c                   6.8270
_cell_volume                     974.236
_database_code_amcsd             0020460
_exptl_crystal_density_diffrn    1.961
_cod_data_source_file            inputs/fixed/downloads/18/18284.cif
_cod_data_source_block           18284
_cod_original_formula_sum        'Zn S O11 H14'
_cod_database_code               9017541
Alumoakermanite, (Ca,Na)2(Al,Mg,Fe2+)(Si2O7), a new mineral from the active carbonatite-nephelinite-phonolite volcano Oldoinyo Lengai, northern Tanzania
Wiedenmann, D.; Zaitsev, A. N.; Britvin, S. N.; Krivovichev, S. V.; Keller, J.; Mineralogical Magazine 73 (2009) 373–384; doi:

data_9017542
_publ_section_title
;
 Alumoakermanite, (Ca,Na)2(Al,Mg,Fe2+)(Si2O7), a new mineral from the active
 carbonatite-nephelinite-phonolite volcano Oldoinyo Lengai, northern Tanzania
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              373
_journal_page_last               384
_journal_volume                  73
_journal_year                    2009
_chemical_compound_source        'Oldoinyo Lengai, northern Tanzania'
_chemical_formula_sum            'Al0.5 Ca1.52 Fe0.3 Mg0.2 Na0.48 O7 Si2'
_chemical_name_mineral           Alumoakermanite
_space_group_IT_number           113
_space_group_name_Hall           'P -4 2ab'
_space_group_name_H-M_alt        'P -4 21 m'
_symmetry_space_group_name_H-M   'P -4 21 m'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_length_a                   7.7661
_cell_length_b                   7.7661
_cell_length_c                   5.0297
_cell_formula_units_Z            2
_cell_volume                     303.353
_database_code_amcsd             0020206
_exptl_crystal_density_diffrn    3.013
_cod_data_source_file            inputs/fixed/downloads/18/18339.cif
_cod_data_source_block           18339
_cod_original_formula_sum        '(Ca1.52 Na.48) (Al.5 Fe.3 Mg.2) Si2 O7'
_cod_database_code               9017542
The crystal chemistry of holtite Sample: H1
Groat, L. A.; Grew, E. S.; Evans, R. J.; Pieczka, A.; Ercit, T. S.; Mineralogical Magazine 73 (2009) 1033–1050; doi:

data_9017543
_publ_section_title
;
 The crystal chemistry of holtite
 Sample: H1
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              1033
_journal_page_last               1050
_journal_volume                  73
_journal_year                    2009
_chemical_compound_source
'Voroni Tundry, Kola Peninsula, Murmanskaja Oblast, Russia'
_chemical_formula_sum            'Al6.32 As0.152 B O17.61 Sb0.238 Si2.61 Ta0.32'
_chemical_name_mineral           Holtite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.6818
_cell_length_b                   11.867
_cell_length_c                   20.302
_cell_formula_units_Z            4
_cell_volume                     1127.957
_database_code_amcsd             0019925
_exptl_crystal_density_diffrn    3.737
_cod_data_source_file            inputs/fixed/downloads/18/18345.cif
_cod_data_source_block           18345
_cod_original_formula_sum        'Al6.32 Ta.32 Si2.61 Sb.238 As.152 B O17.61'
_cod_database_code               9017543
The crystal chemistry of holtite Sample: H2
Groat, L. A.; Grew, E. S.; Evans, R. J.; Pieczka, A.; Ercit, T. S.; Mineralogical Magazine 73 (2009) 1033–1050; doi:

data_9017544
_publ_section_title
;
 The crystal chemistry of holtite
 Sample: H2
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              1033
_journal_page_last               1050
_journal_volume                  73
_journal_year                    2009
_chemical_compound_source
'Greenbushes tinfield, Bridgetown-Greenbushes Shire, Australia'
_chemical_formula_sum            'Al6.39 As0.138 B O17.65 Sb0.21 Si2.65 Ta0.23'
_chemical_name_mineral           Holtite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.6981
_cell_length_b                   11.926
_cell_length_c                   20.413
_cell_formula_units_Z            4
_cell_volume                     1143.731
_database_code_amcsd             0019926
_exptl_crystal_density_diffrn    3.586
_cod_data_source_file            inputs/fixed/downloads/18/18346.cif
_cod_data_source_block           18346
_cod_original_formula_sum        'Al6.39 Ta.23 Si2.65 Sb.21 As.138 B O17.65'
_cod_database_code               9017544
The crystal chemistry of holtite Sample: H3
Groat, L. A.; Grew, E. S.; Evans, R. J.; Pieczka, A.; Ercit, T. S.; Mineralogical Magazine 73 (2009) 1033–1050; doi:

data_9017545
_publ_section_title
;
 The crystal chemistry of holtite
 Sample: H3
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              1033
_journal_page_last               1050
_journal_volume                  73
_journal_year                    2009
_chemical_compound_source
'Greenbushes tinfield, Bridgetown-Greenbushes Shire, Australia'
_chemical_formula_sum
'Al6.374 As0.052 B O17.156 Sb0.792 Si2.156 Ta0.26'
_chemical_name_mineral           Holtite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.6900
_cell_length_b                   11.897
_cell_length_c                   20.385
_cell_formula_units_Z            4
_cell_volume                     1137.420
_database_code_amcsd             0019927
_exptl_crystal_density_diffrn    3.885
_cod_data_source_file            inputs/fixed/downloads/18/18347.cif
_cod_data_source_block           18347
_cod_original_cell_volume        1137.421
_cod_original_formula_sum        'Al6.374 Ta.26 Si2.156 Sb.792 As.052 B O17.156'
_cod_database_code               9017545
The crystal chemistry of holtite Sample: H4
Groat, L. A.; Grew, E. S.; Evans, R. J.; Pieczka, A.; Ercit, T. S.; Mineralogical Magazine 73 (2009) 1033–1050; doi:

data_9017546
_publ_section_title
;
 The crystal chemistry of holtite
 Sample: H4
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              1033
_journal_page_last               1050
_journal_volume                  73
_journal_year                    2009
_chemical_compound_source
'Mt. Szklana Mine, Szklary, Zabkowice, Lower Silesia, Poland'
_chemical_formula_sum            'Al6.54 As0.22 B O17.186 Sb0.62 Si2.186 Ta0.11'
_chemical_name_mineral           Holtite
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.7264
_cell_length_b                   11.981
_cell_length_c                   20.566
_cell_formula_units_Z            4
_cell_volume                     1164.591
_database_code_amcsd             0019928
_exptl_crystal_density_diffrn    3.625
_cod_data_source_file            inputs/fixed/downloads/18/18348.cif
_cod_data_source_block           18348
_cod_original_formula_sum        'Al6.54 Ta.11 Si2.186 Sb.62 As.22 B O17.186'
_cod_database_code               9017546
Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4 tetrahedra in silicates
Nagashima, M.; Armbruster, T.; Mineralogical Magazine 74 (2010) 55–71; doi:

data_9017547
_publ_section_title
;
 Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4
 tetrahedra in silicates
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              55
_journal_page_last               71
_journal_volume                  74
_journal_year                    2010
_chemical_compound_source        'Salm-Chateau, Ardennes, Belgium'
_chemical_formula_sum
'Al5.022 As0.833 Ca0.69 Cu0.07 H6 Mg0.84 Mn3.31 O28 Si5.04 V0.195'
_chemical_name_mineral           Ardennite-(As)
_space_group_IT_number           59
_space_group_name_Hall           '-P 2c 2bc'
_space_group_name_H-M_alt        'P n m m :2'
_symmetry_space_group_name_H-M   'P n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.7163
_cell_length_b                   5.8131
_cell_length_c                   18.5199
_cell_volume                     938.380
_database_code_amcsd             0019900
_exptl_crystal_density_diffrn    3.673
_cod_data_source_file            inputs/fixed/downloads/18/18350.cif
_cod_data_source_block           18350
_cod_original_sg_symbol_H-M      'P n m m'
_cod_original_formula_sum
'(Mn3.31 Ca.69) Al5.022 Mg.84 Cu.07 V.195 Si5.04 As.833 O28 H6'
_cod_database_code               9017547
Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4 tetrahedra in silicates
Nagashima, M.; Armbruster, T.; Mineralogical Magazine 74 (2010) 55–71; doi:

data_9017548
_publ_section_title
;
 Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4
 tetrahedra in silicates
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              55
_journal_page_last               71
_journal_volume                  74
_journal_year                    2010
_chemical_compound_source
'Vernetto mine, Val Lanzo, Torino, Piedmont, Italy'
_chemical_formula_sum
'Al4.314 As0.73 Ca1.26 Fe0.244 H6 Mg1.08 Mn3.102 O28 Si5.27'
_chemical_name_mineral           Ardennite-(As)
_space_group_IT_number           59
_space_group_name_Hall           '-P 2c 2bc'
_space_group_name_H-M_alt        'P n m m :2'
_symmetry_space_group_name_H-M   'P n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.7452
_cell_length_b                   5.8314
_cell_length_c                   18.5891
_cell_formula_units_Z            2
_cell_volume                     947.984
_database_code_amcsd             0019901
_exptl_crystal_density_diffrn    3.622
_cod_data_source_file            inputs/fixed/downloads/18/18351.cif
_cod_data_source_block           18351
_cod_original_sg_symbol_H-M      'P n m m'
_cod_original_formula_sum
'Mn3.102 Ca1.26 Al4.314 Fe.244 Mg1.08 Si5.27 As.73 O28 H6'
_cod_database_code               9017548
Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4 tetrahedra in silicates
Nagashima, M.; Armbruster, T.; Mineralogical Magazine 74 (2010) 55–71; doi:

data_9017549
_publ_section_title
;
 Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4
 tetrahedra in silicates
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              55
_journal_page_last               71
_journal_volume                  74
_journal_year                    2010
_chemical_compound_source        'Gambatesa mine, Val Graveglia, Liguria, Italy'
_chemical_formula_sum            'As0.7 Ca0.062 H Mn3.938 O13 Si3.22 V0.08'
_chemical_name_mineral           Tiragalloite
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.475
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.6783
_cell_length_b                   19.9075
_cell_length_c                   7.5750
_cell_volume                     1002.489
_database_code_amcsd             0019902
_exptl_crystal_density_diffrn    3.808
_cod_data_source_file            inputs/fixed/downloads/18/18352.cif
_cod_data_source_block           18352
_cod_original_formula_sum        'Mn3.938 Ca.062 Si3.22 As.7 V.08 O13 H'
_cod_database_code               9017549
Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4 tetrahedra in silicates
Nagashima, M.; Armbruster, T.; Mineralogical Magazine 74 (2010) 55–71; doi:

data_9017550
_publ_section_title
;
 Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4
 tetrahedra in silicates
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              55
_journal_page_last               71
_journal_volume                  74
_journal_year                    2010
_chemical_compound_source        'Molinello, Val Graveglia, Liguria, Italy'
_chemical_formula_sum            'As0.175 Ca0.15 H Mn5.85 O19 Si5.23 V0.595'
_chemical_name_mineral           Medaite
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.309
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.7079
_cell_length_b                   28.8700
_cell_length_c                   7.5754
_cell_volume                     1460.736
_database_code_amcsd             0019903
_exptl_crystal_density_diffrn    3.741
_cod_data_source_file            inputs/fixed/downloads/18/18353.cif
_cod_data_source_block           18353
_cod_original_cell_volume        1460.737
_cod_original_formula_sum        'Mn5.85 Ca.15 Si5.23 V.595 As.175 O19 H'
_cod_database_code               9017550
Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4 tetrahedra in silicates
Nagashima, M.; Armbruster, T.; Mineralogical Magazine 74 (2010) 55–71; doi:

data_9017551
_publ_section_title
;
 Ardennite, tiragalloite and medaite: structural control of (As5+,V5+,Si4+)O4
 tetrahedra in silicates
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              55
_journal_page_last               71
_journal_volume                  74
_journal_year                    2010
_chemical_compound_source        'Fianel, Val Ferrera, Graubunden, Switzerland'
_chemical_formula_sum            'As0.093 H Mn6 O19 Si5.07 V0.837'
_chemical_name_mineral           Medaite
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.363
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.6748
_cell_length_b                   28.8203
_cell_length_c                   7.5444
_cell_volume                     1444.961
_database_code_amcsd             0019904
_exptl_crystal_density_diffrn    3.800
_cod_data_source_file            inputs/fixed/downloads/18/18354.cif
_cod_data_source_block           18354
_cod_original_formula_sum        'Mn6 Si5.07 V.837 As.093 O19 H'
_cod_database_code               9017551
The crystal structure of dalnegroite, Tl5-xPb2x(As,Sb)21-xS34: a masterpiece of structural complexity
Bindi, L.; Nestola, F.; Guastoni, A.; Secco, L.; Mineralogical Magazine 74 (2013) 999–1012; doi:

data_9017552
_publ_section_title
;
 The crystal structure of dalnegroite, Tl5-xPb2x(As,Sb)21-xS34:
 a masterpiece of structural complexity
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              999
_journal_page_last               1012
_journal_volume                  74
_journal_year                    2013
_chemical_compound_source
'Lengenbach quarry, Binntal, Canton Valais, Switzerland'
_chemical_formula_sum            'As24 Pb4.01 S68 Sb15.99 Tl8'
_chemical_name_mineral           Dalnegroite
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                95.70
_cell_angle_beta                 90.18
_cell_angle_gamma                96.38
_cell_formula_units_Z            2
_cell_length_a                   16.218
_cell_length_b                   42.546
_cell_length_c                   8.58
_cell_volume                     5853.936
_database_code_amcsd             0020126
_exptl_crystal_density_diffrn    4.761
_cod_data_source_file            inputs/fixed/downloads/18/18375.cif
_cod_data_source_block           18375
_cod_original_cell_volume        5853.937
_cod_original_formula_sum        'Tl8 Pb4.01 Sb15.99 As24 S68'
_cod_database_code               9017552
Short-range constraints on chemical and structural variations in bavenite Sample: 2ABAV
Lussier, A. J.; Hawthorne, F. C.; Mineralogical Magazine 75 (2011) 213–239; doi:

data_9017553
_publ_section_title
;
 Short-range constraints on chemical and structural variations in bavenite
 Sample: 2ABAV
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              213
_journal_page_last               239
_journal_volume                  75
_journal_year                    2011
_chemical_compound_source        'Rincon, San Diego County, California'
_chemical_formula_sum            'Al1.179 Be2.811 Ca3.94 H2 Na0.05 O28 Si9.01'
_chemical_name_mineral           Bavenite
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   23.2080
_cell_length_b                   4.9833
_cell_length_c                   19.4266
_cell_formula_units_Z            4
_cell_volume                     2246.733
_database_code_amcsd             0019874
_exptl_crystal_density_diffrn    2.718
_cod_data_source_file            inputs/fixed/downloads/18/18379.cif
_cod_data_source_block           18379
_cod_original_formula_sum        'Na.05 Ca3.94 Si9.01 Be2.811 Al1.179 O28 H2'
_cod_database_code               9017553
Short-range constraints on chemical and structural variations in bavenite Sample: 7BAV
Lussier, A. J.; Hawthorne, F. C.; Mineralogical Magazine 75 (2011) 213–239; doi:

data_9017554
_publ_section_title
;
 Short-range constraints on chemical and structural variations in bavenite
 Sample: 7BAV
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              213
_journal_page_last               239
_journal_volume                  75
_journal_year                    2011
_chemical_compound_source        'Ilimaussaq, Kangerluarsuk Fjord, Greenland'
_chemical_formula_sum            'Al1.481 Be2.46 Ca3.917 H2 Na0.024 O28 Si9.059'
_chemical_name_mineral           Bavenite
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   23.2028
_cell_length_b                   4.9805
_cell_length_c                   19.4290
_cell_formula_units_Z            4
_cell_volume                     2245.245
_database_code_amcsd             0019875
_exptl_crystal_density_diffrn    2.734
_cod_data_source_file            inputs/fixed/downloads/18/18380.cif
_cod_data_source_block           18380
_cod_original_cell_volume        2245.246
_cod_original_formula_sum        'Na.024 Ca3.917 Si9.059 Be2.46 Al1.481 O28 H2'
_cod_database_code               9017554
Short-range constraints on chemical and structural variations in bavenite Sample: 10BAV
Lussier, A. J.; Hawthorne, F. C.; Mineralogical Magazine 75 (2011) 213–239; doi:

data_9017555
_publ_section_title
;
 Short-range constraints on chemical and structural variations in bavenite
 Sample: 10BAV
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              213
_journal_page_last               239
_journal_volume                  75
_journal_year                    2011
_chemical_compound_source        'Government Pit, Albany, New Hampshire'
_chemical_formula_sum
'Al0.598 Be2.811 Ca3.946 H2 Na0.037 O28 Si9.223'
_chemical_name_mineral           Bavenite
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   23.2068
_cell_length_b                   4.9929
_cell_formula_units_Z            4
_cell_length_c                   19.4340
_cell_volume                     2251.803
_database_code_amcsd             0019876
_exptl_crystal_density_diffrn    2.683
_cod_data_source_file            inputs/fixed/downloads/18/18381.cif
_cod_data_source_block           18381
_cod_original_cell_volume        2251.802
_cod_original_formula_sum        'Na.037 Ca3.946 Si9.223 Be2.811 Al.598 O28 H2'
_cod_database_code               9017555
Short-range constraints on chemical and structural variations in bavenite Sample: 11BAV
Lussier, A. J.; Hawthorne, F. C.; Mineralogical Magazine 75 (2011) 213–239; doi:

data_9017556
_publ_section_title
;
 Short-range constraints on chemical and structural variations in bavenite
 Sample: 11BAV
;
_journal_name_full               'Mineralogical Magazine'
_journal_page_first              213
_journal_page_last               239
_journal_volume                  75
_journal_year                    2011
_chemical_compound_source        'Kalisay, Kyrgizstan'
_chemical_formula_sum            'Al1.053 Be2.995 Ca4 H2 Na0.006 O28 Si8.952'
_chemical_name_mineral           Bavenite
_space_group_IT_number           63
_space_group_name_Hall           '-C 2c 2'
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   23.2110
_cell_length_b                   4.9721
_cell_length_c                   19.4189
_cell_formula_units_Z            4
_cell_volume                     2241.085
_database_code_amcsd             0019877
_exptl_crystal_density_diffrn    2.719
_cod_data_source_file            inputs/fixed/downloads/18/18382.cif
_cod_data_source_block           18382
_cod_original_formula_sum        'Na.006 Ca4 Si8.952 Be2.995 Al1.053 O28 H2'
_cod_database_code               9017556